Ternary rare earth silicides RE2M3Si4 (RE = Sc, Y, Lu; M = Mo, W): crystal structure, coloring and electronic properties.
Nielsen, Morten B.; Xie, Weiwei; Cava, Robert J.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 3771–3777; doi:10.1039/c5dt03976b

data_7038100
_publ_section_title
;
 Ternary rare earth silicides RE2M3Si4 (RE = Sc, Y, Lu; M = Mo, W):
 crystal structure, coloring and electronic properties.
;
_journal_issue                   9
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              3771
_journal_page_last               3777
_journal_paper_doi               10.1039/c5dt03976b
_journal_volume                  45
_journal_year                    2016
_chemical_formula_sum            'Sc2.07 Si4 W2.93'
_chemical_formula_weight         744.80
_chemical_name_systematic
; 
 ? 
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_audit_creation_method           SHELXL-2013
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.5357(4)
_cell_length_b                   12.6408(8)
_cell_length_c                   6.7743(4)
_cell_measurement_reflns_used    1963
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      30.53
_cell_measurement_theta_min      3.22
_cell_volume                     559.67(6)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0264
_diffrn_reflns_av_unetI/netI     0.0231
_diffrn_reflns_laue_measured_fraction_full 1.000
_diffrn_reflns_laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            3743
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.538
_diffrn_reflns_theta_min         3.223
_exptl_absorpt_coefficient_mu    63.182
_exptl_absorpt_correction_T_max  0.7461
_exptl_absorpt_correction_T_min  0.4503
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Metallic
_exptl_crystal_density_diffrn    8.839
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'Not measured'
_exptl_crystal_description       Irregular
_exptl_crystal_F_000             1266
_exptl_crystal_size_max          0.020
_exptl_crystal_size_mid          0.015
_exptl_crystal_size_min          0.010
_refine_diff_density_max         1.680
_refine_diff_density_min         -1.870
_refine_diff_density_rms         0.374
_refine_ls_extinction_coef       0.00195(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.138
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     48
_refine_ls_number_reflns         897
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.138
_refine_ls_R_factor_all          0.0232
_refine_ls_R_factor_gt           0.0187
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0154P)^2^+0.1663P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0371
_refine_ls_wR_factor_ref         0.0380
_reflns_Friedel_coverage         0.000
_reflns_number_gt                790
_reflns_number_total             897
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt03976b4.cif
_cod_data_source_block           Sc2.07W2.93Si4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'None' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7038099--7038101.cif.
;
_cod_database_code               7038100
_shelxl_version_number           2013-4
_shelx_res_checksum              43948
_shelx_hkl_checksum              16955